Journal of Nanomaterials

Volume 2014 (2014), Article ID 619239, 6 pages

http://dx.doi.org/10.1155/2014/619239

Research Article

Investigation of Adsorption Behavior of Cu₂O Submicro-Octahedra towards Congo Red

Xu Zhang, Ying Zhang, Dong Wang, and Fengyu Qu

Key Laboratory of Design and Synthesis of Functional Materials and Green Catalysis, Colleges of Heilongjiang Province and College of Chemistry and Chemical Engineering, Harbin Normal University, Harbin, Heilongjiang 150025, China

Received 23 January 2014; Revised 14 March 2014; Accepted 14 March 2014; Published 7 April 2014

Academic Editor: Xiang Wu

Copyright © 2014 Xu Zhang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Perfect cuprous oxide (Cu₂O) nanocrystals with octahedron shape were successfully synthesized by a facile route without chemical additive in a short time. The products were characterized by X-ray diffraction (XRD) and field-emission scanning electron microscopy (FESEM). The adsorption ability of the products towards congo red (CR) as the pollutant was investigated and FTIR spectroscopy was employed to identify the adsorbed species. The adsorption behavior was analyzed based on the microstructure of Cu₂O submicro-octahedra.

1. Introduction

Owing to the close correlations of the surface morphologies and size of inorganic materials with the electronic structure, bonding, surface energy, and chemical reactivity, designing and delicately controlling the shape of nanocrystals is one of the most important issues in nanoscience, chemistry, and physics [1–5]. Therefore, in the past decades, great efforts have been devoted to controllable synthesis of a variety of metal oxides with all types of shapes [6–11]. Among these metal oxides, cuprous oxide has been paid much attention because of its p-type semiconductor nature with a direct band gap of about 2.17 eV and potential application in catalysis, sensors, micro-/nanoelectronics, and solar energy conversion [12–15]. In order to tune the shape of Cu₂O, surfactants were generally used to alter the relative order of the surface energy of different crystallographic facets because of preferential adsorption of them on certain crystallographic surfaces [16–19]. However, the use of surfactants would bring a tedious procedure and lead to an environmental burden to some extent. Therefore, it is highly desirable to develop a facile template-free route to tailored synthesis of Cu₂O nanostructures with highly active facets. The facets with different crystallographic characters have distinctive surface atomic structures, reconstructions, and atomic termination features corresponding to sharp differences that have been demonstrated in chemical reactivity and light-sensing [16, 20–23]. Zhang et al. reported that Cu₂O octahedra exhibited higher adsorption capacity towards methyl orange than Cu₂O cube and cubooctahedra because of the exposure of active “Cu” atoms with dangling bond on the surfaces of Cu₂O octahedra [16]. To date, a variety of methods have been employed to prepare Cu₂O octahedra [24–28]; however, most of these methods involve surfactants or toxic reagent, and some products possess large sizes and low surface areas which is unfavorable to functionalized utilization such as adsorption.

Congo red (C₃₂H₂₂N₆O₆S₂Na₂, CR) is a benzidine-based anionic diazo dye and is widely used in the textiles, printing and dyeing, paper, rubber, plastics industries, and so forth. CR is toxic to animals and plants and thus its introduction to water stream is of potential health, environmental, and ecological concern [29]. Therefore, CR containing effluents have to be adequately treated before they are discharged into the environment. However, CR is difficult to biodegrade owing to its structural stability. Physicochemical or chemical treatment of such wastewater is, however, possible. Adsorption is considered an attractive option in treating such wastewater due to its simple operation, high treatment efficiency, and economy.

Herein, we present a green and simple route to the synthesis of Cu₂O submicro-octahedra with the exposure of active “Cu” atoms with dangling bond in the absence of any surfactant in a short time. In this protocol, only CuCl₂, NaOH, glucose, and distilled water are used, and the product possesses active facets. So it is a highly ideal synthetic route to produce Cu₂O submicro-octahedra under environmentally benign conditions. Moreover, the as-prepared product exhibits good adsorption ability towards congo red, which extends the application of Cu₂O architectures.

2. Experimental Section

2.1. Synthesis of Cu₂O Octahedra

All reagents were of analytical grade and were used in their as-received state. The synthesis of target polyhedral Cu₂O nanocrystals was fulfilled in an alkaline solution using D-(+)-glucose as the reducing agent. In a typical synthesis, firstly, 0.1705 g CuCl₂·2H₂O was dissolved in 17 mL distilled water under constant magnetic stirring. Secondly, 3 mL of NaOH aqueous solution (2.0 mol·L⁻¹) was added to the above solution and blue Cu(OH)₂ precipitates appeared immediately. Thirdly, 0.1982 g D-(+)-glucose was added to the above mixture and magnetically stirred for 2 min. Finally, the mixture was immersed into water bath at 60°C and stirred for 20 min. The precipitates turned from blue into dark yellow, then yellow, and orange in three minutes, which implied the formation of Cu₂O. After the mixture was cooled to room temperature, the precipitates were separated from the solution by centrifugation at 3000 rpm for 3 min. Then the precipitates were washed with distilled water and absolute ethanol for three times and dried in a vacuum oven at 60°C for several hours.

2.2. Characterization

XRD data were collected on a D/max-2600/PC diffractometer with Cu Kα radiation at 40 kV and 150 mA. The morphology and size of these crystals were characterized by scanning electron microscopy (SEM, HITACHI SU-70). The N₂ adsorption-desorption isotherms at 77 K were measured using a Quantachrome NOVA 2000E analyzer. Before being measured, the samples were degassed at 393 K for 12 h. Specific surface area was calculated using the Brunauer-Emmett-Teller (BET) model from the adsorption branch. UV-Vis spectra were taken on a Lambda 45 (Perkin-Elmer) spectrophotometer. Fourier transform infrared spectroscopy (FTIR, Bruker, vertex 80) was employed to characterize the residual CR on the Cu₂O octahedrons after adsorption.

2.3. Adsorption Property Measurement

Different amounts of Cu₂O octahedra (0.05 g–0.15 g) were dispersed into an aqueous solution of congo red (200 mL, 10 mg/L) and the mixed solution was magnetically stirred in the dark. 5 mL of suspension was collected at each regular interval and centrifuged to remove the adsorbent powder in order to analyze the adsorption rate of CR by monitoring dye decolorization at the maximum absorption wavelength, using a Lambda 45 UV/Vis spectrophotometer.

3. Results and Discussion

Figure 1 plots the representative XRD pattern of the as-prepared sample. The sharp peaks in the pattern indicated that the samples obtained by this method were well crystallized. All patterns can be indexed as the cubic phase of cuprous oxide (JCPDS card, number 05-0667). No other characteristic peaks from impurities, such as CuO and Cu, were detected, revealing that the purity of the product was pretty high.

Figure 1: XRD pattern of the as-prepared product.

Figure 2 presents the typical SEM images of a Cu₂O sample prepared in the above-mentioned synthesis process when the reaction time was 20 min. It can be seen that the sample shows uniform and monodisperse octahedral morphology with edge lengths of 300~400 nm. Zhang et al. believed that the surface energy of facet is higher than that of facet due to the exposure of “Cu” atoms with dangling bonds and Cu₂O cubes are easily obtained in the absence of any surfactant [16]. However, in our experiment, the occurrence of Cu₂O octahedra indicated that the surface energy of facet is lower than that of facet. We proposed that it is glucose that plays an important role in the formation of octahedron in the absence of any surfactant. In the reaction, the glucose acts two roles: one is reductant and the other is capping agent. Glucose could be adsorbed preferentially on the surface of facet and the adsorption stabilized the plane, inhibiting the growth rate perpendicular to it. It resulted in the exposure of the surfaces and produced high symmetry octahedra.

(a)

(b)

Figure 2: SEM images of the sample with different magnifications: (a) low magnification image and (b) high magnification image.

To demonstrate the potential application of the as-prepared Cu₂O octahedra, we investigated the adsorption ability of Cu₂O octahedra with congo red (CR, shown in Figure 3) as the pollutant. The experiments were carried out by dispersing different amounts of Cu₂O octahedra in the solution of CR in the dark for various durations under constant stirring. After centrifugation, the UV-Vis absorption of the supernatant was measured and the characteristic absorption of CR at about 496 nm was selected to monitor the adsorption behavior. As illustrated in Figure 4, the same trend can be seen that the concentration of the CR progressively decreases following the adsorption time within 160 min and inclines to be constant beyond 160 min when the dosage of Cu₂O octahedra was in the range 0.05–0.15 g. Obviously, the adsorption capacity of the octahedra is saturated at about 160 min. The more the amount of the octahedra is used, the larger the adsorption rate is. However, the adsorption curves are very close to each other when the used amount of the Cu₂O octahedra is 0.10 g and 0.15 g, and the final adsorption rate could reach about 81% when the adsorption time is 160 min. Obviously, the optimum used amount of the as-prepared adsorbent is around 0.10 g.

Figure 3: Structure of CR (molecular formula: C₃₂H₂₂N₆O₆S₂Na₂).

Figure 4: Adsorption curves of the aqueous solution of congo red (10 mg L⁻¹, 200 mL) in the presence of Cu₂O octahedra (0.05 g–0.15 g) at different intervals, where denotes the concentrations of CR changing following adsorption time and denotes the initial concentration of CR.

Since the adsorption experiments were carried out in the dark, the decolorization of the CR solution must result from the adsorption of Cu₂O particles, which is further corroborated by the FTIR analysis. As shown by curve a in Figure 5, the FTIR spectrum of the Cu₂O octahedra before adsorption exhibits two strong vibration bands. The band at 632 cm⁻¹ corresponds to the Cu–O bond [30] (optically active lattice vibration in the oxide), and the peak at 1628 cm⁻¹ is attributed to the –OH bending vibration [31], which originates from the surface-adsorbed H₂O. In comparison with the FTIR spectrum of the pure Cu₂O octahedra, some new absorption bands appear after adsorption (curve b in Figure 5). Combined with the FTIR spectrum of pure CR (curve c in Figure 5), the new absorption bands can be assigned to the characteristic vibrations of CR. The absorption band at 3458 cm⁻¹ (Figure 5(c)), corresponding to the stretching vibration of –N–H in the structure of dye CR, shifted to lower wave number 3436 cm⁻¹ after adsorption with Cu₂O octahedra (Figure 5(b)). The broadened band at 1575 cm⁻¹ was assigned to –N=N– stretching vibration of CR. The bands at 1409 and 829 cm⁻¹ were assigned to characteristic absorption vibrations of aromatic skeletal groups. The band at 1051 cm⁻¹ was attributed to S=O stretching vibration [32]. Thus, the FTIR characterization results provide solid evidence for the adsorption of CR on the Cu₂O octahedra.

Figure 5: The FTIR spectra of (a) Cu₂O octahedra, (b) Cu₂O octahedra after the CR adsorption, and (c) the pure CR.

The specific surface area of the as-prepared Cu₂O octahedra is calculated to be 3.622 m² g⁻¹ by the Brunauer-Emmett-Teller (BET) model from the sorption isotherms. Obviously, the specific surface area seems too little for the relatively high adsorption capacity. We proposed that the microstructure of the Cu₂O octahedra may play an important role in the adsorption of organic pollutant. For cuprite structured Cu₂O, each “O” is surrounded by a tetrahedron of “Cu”, and each “Cu” has two “O” neighbors as illustrated by its unit cell model (Figure 6(a)). The atomic arrangements along different crystallographic planes of Cu₂O are displayed in Figures 6(b) to 6(d). Structurally, the cuprite Cu₂O crystal can be described as layers of atoms stacking alternately and periodically. Along the [100] and [110] directions (Figures 6(b) and 6(c)), the periodicity can be defined as two layers, in principle, layer 1 and layer 2 have equal possibility as a termination layer in both of these two cases. However, since the growth took place in aqueous media, “Cu”-terminated (layer 1 in Figure 6(b) and layer 1 in Figure 6(c)) would be rather unstable due to the active interaction with the hydroxyl group. Thus, “O”-(layer 2 in Figure 6(b)) and “–O–Cu–O–Cu–”-(layer 2 in Figure 6(c)) terminated surfaces are expected for and planes, respectively [16]. With respect to the [111] direction, three atom layers consist of one period, where the “Cu” layer is sandwiched between two layers of “O” atoms (Figure 6(d)). However, the distance between two adjacent layers in such a period is so short that the three layers can be approximately regarded as in the same surface. Every two “Cu” atoms have a dangling bond perpendicular to the planes [16]. CR is an anionic dye with two negative charges in a molecule. The active “Cu” atoms with dangling bond in the surfaces of Cu₂O octahedra tend to interact with negatively charged CR (i.e., ) to compensate the local surface charge imbalance. Based on the above discussion, we proposed that the interaction between Cu₂O octahedra and CR is not simple physical adsorption.

(a)

(b)

(c)

(d)

Figure 6: (a) The unit cell of the cuprite Cu₂O structure. The blue spheres represent copper atoms and yellow spheres indicate oxygen atoms. ((b)–(d)) The atomic arrangements in the (100), (110), and (111) planes of the Cu₂O structure, respectively.

4. Conclusions

In summary, we have successfully synthesized octahedral morphology Cu₂O nanocrystals with edge length of 300~400 nm using glucose as the reducing agent via a facile procedure, where glucose also acts as capping agent to control the growth of octahedra. The as-prepared Cu₂O submicro-octahedra exhibit good absorption ability towards CR due to the exposure of active “Cu” atoms with dangling bond on the surfaces.

Conflict of Interests

The authors declare that there is no conflict of interests regarding the publication of this paper.

Acknowledgment

This work was financially supported by the Scientific Research Fund of Heilongjiang provincial Education Department (no. 1155G27).

References

A. R. Tao, S. Habas, and P. Yang, “Shape control of colloidal metal nanocrystals,” Small, vol. 4, no. 3, pp. 310–325, 2008.

N. Tian, Z.-Y. Zhou, S.-G. Sun, Y. Ding, and L. W. Zhong, “Synthesis of tetrahexahedral platinum nanocrystals with high-index facets and high electro-oxidation activity,” Science, vol. 316, no. 5825, pp. 732–735, 2007.

H. Xu, W. Wang, and W. Zhu, “Shape evolution and size-controllable synthesis of Cu₂O octahedra and their morphology-dependent photocatalytic properties,” Journal of Physical Chemistry B, vol. 110, no. 28, pp. 13829–13834, 2006.

J. Chen, B. J. Wiley, and Y. Xia, “One-dimensional nanostructures of metals: large-scale synthesis and some potential applications,” Langmuir, vol. 23, no. 8, pp. 4120–4129, 2007.

D. Seo, C. I. Yoo, J. C. Park, S. M. Park, S. Ryu, and H. Song, “Directed surface overgrowth and morphology control of polyhedral gold nanocrystals,” Angewandte Chemie International Edition, vol. 47, no. 4, pp. 763–767, 2008.

Y. Jiao, Y. Liu, F. Y. Qu, and X. Wu, “Dendritic α-Fe₂O₃ hierarchical architectures for visible light driven photocatalysts,” CrystEngComm, vol. 16, no. 4, pp. 575–580, 2014.

Y. Han, X. Wu, Y. Ma, L. Gong, F. Qu, and H. Fan, “Porous SnO₂ nanowire bundles for photocatalyst and Li ion battery applications,” CrystEngComm, vol. 13, no. 10, pp. 3506–3510, 2011.

B. X. Jia, W. N. Jia, F. Y. Qu, and X. Wu, “General strategy for self assembly of mesoporous SnO₂ nanospheres and their applications in water purification,” RSC Advances, vol. 3, no. 30, pp. 12140–12148, 2013.

J. Wang, F. Y. Qu, and X. Wu, “Synthesis of ultra-thin ZnO nanosheets: photocatalytic and superhydrophilic properties,” Science of Advanced Materials, vol. 5, no. 8, pp. 1052–1059, 2013.

J. Wang, F. Y. Qu, and X. Wu, “Photocatalytic degradation of organic dyes with hierarchical Ag₂O/ZnO heterostructures under simulated sunlight irradiation,” Science of Advanced Materials, vol. 5, no. 10, pp. 1364–1371, 2013.

Y. Zhang, D. Wang, X. Zhang, and F. Y. Qu, “Template-free synthesis of porous Cu₂O nanospheres at room temperature and investigation on their adsorption property,” Journal of Nanomaterials, vol. 2013, Article ID 378919, 5 pages, 2013.

M. Leng, M. Liu, Y. Zhang et al., “Polyhedral 50-facet Cu₂O microcrystals partially enclosed by high-index planes: synthesis and enhanced catalytic CO oxidation activity,” Journal of the American Chemical Society, vol. 132, no. 48, pp. 17084–17087, 2010.

L. Guan, H. Pang, J. Wang, Q. Lu, J. Yin, and F. Gao, “Fabrication of novel comb-like Cu₂O nanorod-based structures through an interface etching method and their application as ethanol sensors,” Chemical Communications, vol. 46, no. 37, pp. 7022–7024, 2010.

A. Chen, S. Haddad, Y. C. Wu, T. N. Fang, S. Kaza, and Z. Lan, “Erasing characteristics of Cu₂O metal-insulator-metal resistive switching memory,” Applied Physics Letters, vol. 92, no. 1, Article ID 013503, 2008.

S. K. Baek, K. R. Lee, and H. K. Cho, “Oxide p-n heterojunction of Cu₂O/ZnO nanowires and their photovoltaic performance,” Journal of Nanomaterials, vol. 2013, Article ID 421371, 7 pages, 2013.

D.-F. Zhang, H. Zhang, L. Guo, K. Zheng, X.-D. Han, and Z. Zhang, “Delicate control of crystallographic facet-oriented Cu₂O nanocrystals and the correlated adsorption ability,” Journal of Materials Chemistry, vol. 19, no. 29, pp. 5220–5225, 2009.

W.-C. Huang, L.-M. Lyu, Y.-C. Yang, and M. H. Huang, “Synthesis of Cu₂O nanocrystals from cubic to rhombic dodecahedral structures and their comparative photocatalytic activity,” Journal of the American Chemical Society, vol. 134, no. 2, pp. 1261–1267, 2012.

X. Liang, L. Gao, S. Yang, and J. Sun, “Facile synthesis and shape evolution of single-crystal cuprous oxide,” Advanced Materials, vol. 21, no. 20, pp. 2068–2071, 2009.

C.-H. Kuo and M. H. Huang, “Morphologically controlled synthesis of Cu₂O nanocrystals and their properties,” Nano Today, vol. 5, no. 2, pp. 106–116, 2010.

L. Song, Y. Zhang, X. Wu et al., “One-step synthesis of crystalline anatase TiO₂ nanospindles and investigation on their photocatalytic performance,” Materials Letters, vol. 100, pp. 198–200, 2013.

L. Pan, J.-J. Zou, S. Wang, X.-Y. Liu, X. Zhang, and L. Wang, “Morphology evolution of TiO₂ facets and vital influences on photocatalytic activity,” ACS Applied Materials and Interfaces, vol. 4, no. 3, pp. 1650–1655, 2012.

K. Chanda, S. Rej, and M. H. Huang, “Facet-dependent catalytic activity of Cu₂O nanocrystals in the one-pot synthesis of 1, 2, 3-triazoles by multicomponent click reactions,” Chemistry, vol. 19, no. 47, pp. 16036–16043, 2013.

K. H. Schulz and D. F. Cox, “Propene oxidation over Cu₂O single-crystal surfaces: a surface science study of propene activation at 1 atm and 300 K,” Journal of Catalysis, vol. 143, no. 2, pp. 464–480, 1993.

W. Zhai, F. Q. Sun, W. Chen, L. H. Zhang, Z. L. Min, and W. S. Li, “Applications of Cu₂O octahedral particles on ITO glass in photocatalytic degradation of dye pollutants under a halogen tungsten lamp,” Materials Research Bulletin, vol. 48, no. 11, pp. 4953–4959, 2013.

P. McFadyen and E. Matijević, “Copper hydrous oxide sols of uniform particle shape and size,” Journal of Colloid And Interface Science, vol. 44, no. 1, pp. 95–106, 1973.

Y. Dong, Y. Li, C. Wang, A. Cui, and Z. Deng, “Preparation of cuprous oxide particles of different crystallinity,” Journal of Colloid and Interface Science, vol. 243, no. 1, pp. 85–89, 2001.

Y. Cao, Y. J. Wang, K. G. Zhou, and Z. Bi, “Morphology control of ultrafine cuprous oxide powder and its growth mechanism,” Transcations of Nonferrous Metals Society of China, vol. 20, supplement 1, pp. s216–s220, 2010.

Y. J. Wang and K. G. Zhou, “Effect of OH− on morphology of Cu₂O particles prepared through reduction of Cu(II) by glucose,” Journal of Central South University, vol. 19, no. 8, pp. 2125–2129, 2012.

R. Ahmad and R. Kumar, “Adsorptive removal of congo red dye from aqueous solution using bael shell carbon,” Applied Surface Science, vol. 257, no. 5, pp. 1628–1633, 2010.

Z. C. Orel, A. Anžlovar, G. Dražić, and M. Žigon, “Cuprous oxide nanowires prepared by an additive-free polyol process,” Crystal Growth & Design, vol. 7, no. 2, pp. 453–458, 2007.

W. Jiang, J. Joens, D. D. Dionysiou, and K. E. O'Shea, “Optimization of photocatalytic performance of TiO₂ coated glass microspheres using response surface methodology and the application for degradation of dimethyl phthalate,” Journal of Photochemistry and Photobiology A: Chemistry, vol. 262, pp. 7–13, 2013.

L. Wang and A. Wang, “Adsorption properties of Congo Red from aqueous solution onto surfactant-modified montmorillonite,” Journal of Hazardous Materials, vol. 160, no. 1, pp. 173–180, 2008.